Solvent-free synthesis of new magnesium phosphate‒oxalates displaying diverse framework topologies
Zhang, Wei; Kang, Maoping; Yang, Meng; Luo, Daibing; Lin, Zhien; CrystEngComm 17 (2015) 9296–; doi:10.1039/C5CE02001H

data_7223196
_publ_section_title
;
 Solvent-free synthesis of new magnesium phosphate--oxalates displaying
 diverse framework topologies
;
_journal_issue                   48
_journal_name_full               CrystEngComm
_journal_page_first              9296
_journal_paper_doi               10.1039/C5CE02001H
_journal_volume                  17
_journal_year                    2015
_chemical_absolute_configuration unk
_chemical_formula_moiety         'C8 H5 Mg4 O28 P3, 2(H2 O), 2(C4 H12 N2)'
_chemical_formula_sum            'C16 H33 Mg4 N4 O30 P3'
_chemical_formula_weight         951.61
_space_group_crystal_system      triclinic
_space_group_IT_number           1
_space_group_name_Hall           'P 1'
_space_group_name_H-M_alt        'P 1'
_symmetry_space_group_name_Hall  'P 1'
_symmetry_space_group_name_H-M   'P 1'
_atom_sites_solution_hydrogens   mixed
_atom_sites_solution_primary     direct
_audit_creation_date             2015-08-19
_audit_creation_method
;
Olex2 1.2
(compiled 2015.01.26 svn.r3150 for OlexSys, GUI svn.r4998)
;
_audit_update_record
;
2015-10-13 deposited with the CCDC.
2015-11-10 downloaded from the CCDC.
;
_cell_angle_alpha                78.102(3)
_cell_angle_beta                 78.574(4)
_cell_angle_gamma                86.183(3)
_cell_formula_units_Z            1
_cell_length_a                   7.7738(3)
_cell_length_b                   9.4840(3)
_cell_length_c                   11.9243(5)
_cell_measurement_reflns_used    6096
_cell_measurement_temperature    293.15
_cell_measurement_theta_max      72.5240
_cell_measurement_theta_min      4.7520
_cell_volume                     842.90(6)
_computing_cell_refinement
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.33 (release 27-03-2014 CrysAlis171 .NET)
(compiled Mar 27 2014,17:12:48)
;
_computing_data_collection
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.33 (release 27-03-2014 CrysAlis171 .NET)
(compiled Mar 27 2014,17:12:48)
;
_computing_data_reduction
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.33 (release 27-03-2014 CrysAlis171 .NET)
(compiled Mar 27 2014,17:12:48)
;
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2008)'
_computing_structure_solution    'ShelXT (Sheldrick, 2015)'
_diffrn_ambient_temperature      293.15
_diffrn_detector                 'CCD plate'
_diffrn_detector_area_resol_mean 15.9595
_diffrn_detector_type            EosS2
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_details
;
  1 omega   18.00  106.00   1.0000    1.0000
omega____ theta____ kappa____ phi______ frames
    -       36.5421   38.0000   30.0000 88

  2 omega   23.00   90.00   1.0000    1.0000
omega____ theta____ kappa____ phi______ frames
    -       36.5421 -125.0000   60.0000 67

  3 omega    1.00   75.00   1.0000    1.0000
omega____ theta____ kappa____ phi______ frames
    -       36.5421  -99.0000 -150.0000 74

  4 omega  -31.00   53.00   1.0000    1.0000
omega____ theta____ kappa____ phi______ frames
    -       36.5421  -57.0000  150.0000 84

  5 omega  -33.00   55.00   1.0000    1.0000
omega____ theta____ kappa____ phi______ frames
    -       36.5421  -38.0000   60.0000 88

  6 omega   20.00  104.00   1.0000    1.0000
omega____ theta____ kappa____ phi______ frames
    -       36.5421   57.0000 -120.0000 84

  7 omega   20.00  104.00   1.0000    1.0000
omega____ theta____ kappa____ phi______ frames
    -       36.5421   57.0000  -60.0000 84

  8 omega   23.00   90.00   1.0000    1.0000
omega____ theta____ kappa____ phi______ frames
    -       36.5421 -125.0000  150.0000 67

  9 omega   40.00  135.00   1.0000    3.0000
omega____ theta____ kappa____ phi______ frames
    -      108.0000  -77.0000    0.0000 95

 10 omega   39.00  109.00   1.0000    3.0000
omega____ theta____ kappa____ phi______ frames
    -      108.0000  -94.0000  -90.0000 70

 11 omega   38.00   91.00   1.0000    3.0000
omega____ theta____ kappa____ phi______ frames
    -      108.0000  -30.0000  -90.0000 53

 12 omega   90.00  175.00   1.0000    3.0000
omega____ theta____ kappa____ phi______ frames
    -      108.0000   61.0000   60.0000 85

 13 omega   38.00   91.00   1.0000    3.0000
omega____ theta____ kappa____ phi______ frames
    -      108.0000  -30.0000    0.0000 53

 14 omega   38.00  116.00   1.0000    3.0000
omega____ theta____ kappa____ phi______ frames
    -      108.0000 -111.0000 -180.0000 78

 15 omega  100.00  178.00   1.0000    3.0000
omega____ theta____ kappa____ phi______ frames
    -      108.0000  111.0000  -30.0000 78

 16 omega   40.00   98.00   1.0000    3.0000
omega____ theta____ kappa____ phi______ frames
    -      108.0000  -45.0000  120.0000 58

 17 omega   37.00  146.00   1.0000    3.0000
omega____ theta____ kappa____ phi______ frames
    -      108.0000  -15.0000   30.0000 109

 18 omega   39.00  109.00   1.0000    3.0000
omega____ theta____ kappa____ phi______ frames
    -      108.0000  -94.0000  -30.0000 70

 19 omega   40.00   98.00   1.0000    3.0000
omega____ theta____ kappa____ phi______ frames
    -      108.0000  -45.0000  150.0000 58

 20 omega   41.00  126.00   1.0000    3.0000
omega____ theta____ kappa____ phi______ frames
    -      108.0000  -61.0000  -30.0000 85

 21 omega   38.00   91.00   1.0000    3.0000
omega____ theta____ kappa____ phi______ frames
    -      108.0000  -30.0000 -120.0000 53

 22 omega   91.00  176.00   1.0000    3.0000
omega____ theta____ kappa____ phi______ frames
    -      108.0000   45.0000   30.0000 85

 23 omega    0.00   26.00   1.0000    1.0000
omega____ theta____ kappa____ phi______ frames
    -       36.5421   94.0000   83.6219 26

 24 omega  -33.00   55.00   1.0000    1.0000
omega____ theta____ kappa____ phi______ frames
    -       36.5421  -38.0000  -60.0000 88

 25 omega   20.00  104.00   1.0000    1.0000
omega____ theta____ kappa____ phi______ frames
    -       36.5421   57.0000  120.0000 84

 26 omega   20.00  104.00   1.0000    1.0000
omega____ theta____ kappa____ phi______ frames
    -       36.5421   57.0000 -180.0000 84

 27 omega   10.00  104.00   1.0000    1.0000
omega____ theta____ kappa____ phi______ frames
    -       36.5421   77.0000    0.0000 94

 28 omega   10.00  104.00   1.0000    1.0000
omega____ theta____ kappa____ phi______ frames
    -       36.5421   77.0000 -150.0000 94

 29 omega  -33.00   55.00   1.0000    1.0000
omega____ theta____ kappa____ phi______ frames
    -       36.5421  -38.0000 -150.0000 88

 30 omega   87.00  134.00   1.0000    3.0000
omega____ theta____ kappa____ phi______ frames
    -      108.0000   30.0000  120.0000 47

 31 omega   70.00  178.00   1.0000    3.0000
omega____ theta____ kappa____ phi______ frames
    -      108.0000   15.0000 -150.0000 108
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'New Gemini, Dual, Cu at zero, EosS2'
_diffrn_measurement_method       '\w scans'
_diffrn_orient_matrix_UB_11      0.1072330000
_diffrn_orient_matrix_UB_12      -0.0393027000
_diffrn_orient_matrix_UB_13      0.0982980000
_diffrn_orient_matrix_UB_21      0.1708526000
_diffrn_orient_matrix_UB_22      0.0055004000
_diffrn_orient_matrix_UB_23      -0.0917303000
_diffrn_orient_matrix_UB_31      0.0147202000
_diffrn_orient_matrix_UB_32      0.1612527000
_diffrn_orient_matrix_UB_33      -0.0002347000
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54184
_diffrn_reflns_av_R_equivalents  0.0315
_diffrn_reflns_av_unetI/netI     0.0429
_diffrn_reflns_laue_measured_fraction_full 0.999
_diffrn_reflns_laue_measured_fraction_max 0.999
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -7
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            9059
_diffrn_reflns_point_group_measured_fraction_full 0.768
_diffrn_reflns_point_group_measured_fraction_max 0.768
_diffrn_reflns_theta_full        67.002
_diffrn_reflns_theta_max         67.002
_diffrn_reflns_theta_min         4.767
_diffrn_source                   'Enhance (Cu) X-ray Source'
_exptl_absorpt_coefficient_mu    3.482
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.82932
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.33 (release 27-03-2014 CrysAlis171 .NET)
(compiled Mar 27 2014,17:12:48)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            'clear colourless'
_exptl_crystal_colour_lustre     clear
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    1.875
_exptl_crystal_F_000             490
_exptl_crystal_size_max          0.46
_exptl_crystal_size_mid          0.28
_exptl_crystal_size_min          0.24
_refine_diff_density_max         0.464
_refine_diff_density_min         -0.537
_refine_diff_density_rms         0.103
_refine_ls_abs_structure_details
;
 Flack x determined using 1535 quotients [(I+)-(I-)]/[(I+)+(I-)]
 (Parsons, Flack and Wagner, Acta Cryst. B69 (2013) 249-259).
;
_refine_ls_abs_structure_Flack   0.163(16)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.065
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     522
_refine_ls_number_reflns         4630
_refine_ls_number_restraints     3
_refine_ls_restrained_S_all      1.065
_refine_ls_R_factor_all          0.0480
_refine_ls_R_factor_gt           0.0473
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0944P)^2^+0.2047P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1243
_refine_ls_wR_factor_ref         0.1257
_reflns_Friedel_coverage         0.537
_reflns_friedel_fraction_full    0.536
_reflns_friedel_fraction_max     0.536
_reflns_number_gt                4552
_reflns_number_total             4630
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c5ce02001h2.cif
_cod_data_source_block           1
_cod_depositor_comments
'Adding full bibliography for 7223190--7223197.cif.'
_cod_database_code               7223196
_reflns_odcompleteness_completeness 99.93
_reflns_odcompleteness_iscentric 1
_reflns_odcompleteness_theta     66.97
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H,H) groups, All N(H,H) groups
 At 1.5 times of:
  All O(H) groups, All O(H,H) groups
2.a Riding coordinates:
 OW1(HW1A,HW1B)
2.b Free rotating group:
 OW2(HW2A,HW2B)
2.c Secondary CH2 refined with riding coordinates:
 N1(H1A,H1B), N2(H2A,H2B), N3(H3A,H3B), N4(H4A,H4B), C9(H9A,H9B), C10(H10A,
 H10B), C11(H11A,H11B), C12(H12A,H12B), C13(H13A,H13B), C14(H14A,H14B),
 C15(H15A,H15B), C16(H16A,H16B)
2.d Idealised tetrahedral OH refined as rotating group:
 O3(H3), O4(H4), O8(H8), O11(H11), O12(H12)
;
_shelx_res_checksum              90533
_shelx_shelxl_version_number     2014/7
_olex2_submission_special_instructions 'No special instructions were received'